#------------------------------------------------------------------------------
#$Date: 2016-02-18 14:25:00 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176728 $
#$URL: svn://www.crystallography.net/cod/cif/8/10/16/8101670.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_8101670
loop_
_publ_author_name
'Eggenweiler, U.'
'Keller, E.'
'Krämer, V.'
'Meyer, C.A.'
'Ketterer, J.'
_publ_section_title
;
Crystal structure of tribismuth tetraoxide chloride, Bi₃O₄Cl
;
_journal_issue                   4
_journal_name_full
'Zeitschrift für Kristallographie - New Crystal Structures'
_journal_page_first              695
_journal_page_last               695
_journal_volume                  213
_journal_year                    1998
_chemical_formula_sum            'Bi12 Cl4 O16'
_chemical_formula_weight         2905.56
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-I 2ya'
_symmetry_space_group_name_H-M   'I 1 2/a 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 91.5230(8)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   5.6954(4)
_cell_length_b                   5.6476(8)
_cell_length_c                   18.573(2)
_cell_measurement_temperature    293(2)
_cell_volume                     597.19(11)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    8.079
_refine_ls_R_factor_obs          0.0494
_refine_ls_wR_factor_obs         0.1091
_cod_original_sg_symbol_H-M      'I 2/a'
_cod_database_code               8101670
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x, -y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
Bi1 Bi 0.2500 0.7075(2) 0.0000 0.0111(3) Uani 1 d S .
Bi2 Bi 0.21341(13) 0.20782(15) 0.14661(4) 0.0102(3) Uani 1 d . .
Cl1 Cl 0.7500 0.2500 0.2500 0.023(2) Uani 1 d S .
O1 O 0.4857(28) 0.0381(32) 0.0931(8) 0.015(3) Uani 1 d . .
O2 O 0.5857(32) 0.5663(33) 0.0651(10) 0.020(4) Uani 1 d . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 O2 2.19(2) 5_665 ?
Bi1 O2 2.19(2) 6_565 ?
Bi1 O2 2.37(2) 2 ?
Bi1 O2 2.37(2) . ?
Bi1 O1 2.73(2) 5_665 ?
Bi1 O1 2.73(2) 6_565 ?
Bi1 O1 2.86(2) 1_565 ?
Bi1 O1 2.86(2) 2_565 ?
Bi1 Bi1 3.688(2) 5_565 ?
Bi1 Bi1 3.688(2) 5_665 ?
Bi1 Bi2 3.7719(8) 6_665 ?
Bi1 Bi2 3.7719(8) 5_565 ?
Bi2 O2 2.10(2) 6_565 ?
Bi2 O1 2.10(2) . ?
Bi2 O1 2.13(2) 6 ?
Bi2 Cl1 3.2241(9) 4_545 ?
Bi2 Bi2 3.6905(11) 6 ?
Bi2 Bi2 3.6905(11) 6_655 ?
Bi2 Bi1 3.7719(8) 5_565 ?
Bi2 Bi2 3.8813(15) 7 ?
Bi2 Bi1 3.9333(13) 1_545 ?
Cl1 Bi2 3.2241(9) 6_655 ?
Cl1 Bi2 3.2241(9) 4 ?
O1 Bi2 2.13(2) 6_655 ?
O1 Bi1 2.73(2) 5_665 ?
O1 Bi1 2.86(2) 1_545 ?
O2 Bi2 2.10(2) 6_665 ?
O2 Bi1 2.19(2) 5_665 ?
